Catalytic pyrolysis of Laminaria japonica over nanoporous catalysts using Py-GC/MS
© Lee et al; licensee Springer. 2011
Received: 21 May 2011
Accepted: 18 August 2011
Published: 18 August 2011
The catalytic pyrolysis of Laminaria japonica was carried out over a hierarchical meso-MFI zeolite (Meso-MFI) and nanoporous Al-MCM-48 using pyrolysis gas chromatography/mass spectrometry (Py-GC/MS). The effect of the catalyst type on the product distribution and chemical composition of the bio-oil was examined using Py-GC/MS. The Meso-MFI exhibited a higher activity in deoxygenation and aromatization during the catalytic pyrolysis of L. japonica. Meanwhile, the catalytic activity of Al-MCM-48 was lower than that of Meso-MFI due to its weak acidity.
KeywordsLaminaria japonica hierarchical meso-MFI zeolite Al-MCM-48 Py-GC/MS
The importance of alternative energy development has increased rapidly due to high international crude oil price. Therefore, many studies have been reported about producing bioenergy using various biomasses [1–6]. Among them, seaweeds are attractive biomass for fuel production, with higher production rates than land biomass due to their high photosynthesis efficiency . When cultivated in the sea, seaweeds do not require water, land, or fertilizers, which reduces the cost and energy input. Producing biofuels and utilizing seaweeds residues reduce greenhouse gas emissions, as long as such activities do not disturb the food supply and marine ecosystem. Pyrolysis is one option for processing biomass for the production of feedstock and fuel [1–6]. The bio-oils produced via seaweeds pyrolysis can be used as heating fuel, but the fuel quality is low due to its high oxygen content . In terms of importance of seaweeds as a potential source of biofuel, investigation on upgrading of seaweed-derived bio-oil would be very necessary. Even though researches of catalytic upgrading of bio-oil from micro-algae such as Botryococcus braunii, Chlorella, Chaetoceros, Dunaliella, Nannochloropsis, and Spirulina have been reported , the study of upgrading of bio-oil from seaweed has hardly been considered. Among various seaweeds, Laminaria japonica is a representative brown seaweed in East Asia. For example, the annual production of L. japonica is estimated to be 58 kt/year on a dry basis in 2008 in Korea . Therefore, the study of upgrading bio-oil from L. japonica is highly desirable.
To enhance the quality of bio-oil, catalytic pyrolysis over microporous zeolites and nanoporous catalysts has been known to be very promising methods [8–13]. For the catalytic pyrolysis of biomass, it is desirable to apply nanoporous catalysts such as MCM-48 whose pore sizes are around 2 to 6 nm rather than microporous zeolite whose pore size is below 1 nm because nanoporous catalysts are advantageous for the decomposition of high molecular weight species due to their large pore size [11–15]. Also, the highly acidic catalyst would be better due to its high cracking ability. It has been reported that the catalytic activity of zeolites in cracking of hydrocarbons or biomass is correlated with their acidity [16–20]. In both terms of pore size and acidity, the more recently developed hierarchical meso-MFI zeolites (Meso-MFI) are suggested to apply for the catalytic pyrolysis of biomass due to its characteristics of high acidity and nanopore size [9, 10].
Pyrolysis gas chromatography/mass spectrometry (Py-GC/MS) technique is a powerful tool to allow the direct analysis of the pyrolytic products. The product distribution after the catalytic reaction can be compared to reveal the catalytic effects of different catalysts. Furthermore, the chromatographic peak area of a compound is considered to be linear with respect to its quantity, and the peak area percent with its content. If the masses of the biomass and catalyst were the same during each experiment, the corresponding chromatographic peak area percent can be compared to show the change in the relative content of the pyrolysis vapors [6, 13].
In this study, catalytic pyrolysis of L. japonica was investigated over nanoporous catalysts such as Meso-MFI and Al-MCM-48 for the first time. Their catalytic activities were analyzed in terms of the catalytic acidity and pore size.
Synthesis of catalyst
The MCM-48 was prepared using the following procedure . First, to prepare pure MCM-48, 10.0 g of cetyltrimethylammonium bromide, 1.5 g of Brij-30, and 190.5 g of distilled water were mixed. After the mixture became transparent, 46.13 g of a sodium silicate solution (Na/Si = 0.5) was slowly added dropwise under stirring. The prepared solution was reacted in a 100°C oven for 48 h, removed, and allowed to cool. Then, its pH was adjusted to 10 using 50 wt.% acetic acid, and the solution again reacted for another 48 h. The pH adjusting process was repeated three times. The solution was then washed with distilled water, filtered, and dried in the oven for 24 h. This was followed by another washing with ethanol and filtering, and again dried for 24 h and baked at 550°C for 4 h. Aluminum incorporation into MCM-48 was performed using the post-synthetic grafting method . Before baking, the prepared MCM-48 was introduced into a solution prepared by dissolving AlCl3 in 100 mL of ethanol, according to the desired Si/Al ratio, and then stirred for 24 h, washed with ethanol, filtered, dried for 24 h, and calcined for 4 h at 550°C.
A Meso-MFI with a Si/Al molar ratio of 20 was synthesized using a procedure described elsewhere [9, 10]. An amphiphilic organosilane, [(3-trimethoxysilyl)propyl]hexadecyldimethylammonium chloride, was used as a nanopore-directing agent. The catalyst thus obtained was calcined, ion-exchanged with a 1.0 M ammonium nitrate solution at 80°C repeatedly (four times) to convert it into the NH4 + form, and finally calcined again at 550°C to convert it into the H+ form.
Characterization of catalyst
The powder X-ray diffraction (XRD) patterns were determined by X-ray diffractometer (Rigaku D/MAX-III) using Cu-Kα radiation. The Brunauer, Emmett, and Teller (BET) surface area of the catalyst was measured using an ASAP 2010 apparatus (Micromeritics, Norcross, GA, USA). The catalyst sample was dried, with 0.3 g of the dried sample taken, and outgassing under vacuum for 5 h at 250°C using nitrogen as an adsorption gas at the temperature of liquid nitrogen. The nitrogen adsorption-desorption isotherms and BET surface area were then obtained. The surface acidity of the catalysts was measured using temperature programmed desorption of ammonia (NH3-TPD) employing a BEL-CAT TPD analyzer with a TCD detector (BEL Japan Inc., Osaka, Japan). The Si/Al ratio of catalyst was verified by inductively coupled plasma atomic emission spectrometry (ICP-AES, Spectro Ciros Vision, PECTRO Analytical Instruments, Kleve, Germany). For measurements, sample (50 mg) was dissolved with nitrohydrochloric acid (5 ml) using a microwave oven. The decomposed solution was transferred through filter paper into a 100-ml calibrated flask, and the volume was adjusted to 100 ml with ultra-pure water.
A double-shot pyrolyzer (Py-2020iD, Frontier Laboratories Ltd., Koriyama, Fukushima, Japan), coupled directly to GC/MS, was used for identification of the catalytic cracking products. For the sample preparation, the L. japonica (2 mg) and catalyst (1 mg) were placed in a sample cup and then into a 500°C furnace under a He atmosphere. The gaseous species generated during the catalytic cracking were directly introduced into a GC inlet port (split ratio of 1/100) and onto a metal capillary column (Ultra ALLOY-5MS/HT; 5% diphenyl and 95% dimethylpolysiloxane, length 30 m, i.d. 0.25 mm, film thickness 0.5 μm, Frontier Laboratories Ltd.). To prevent condensation of products, the interface and inlet temperatures were both maintained at 300°C. The column temperature was programmed to change from 40°C (5 min) to 320°C (10 min), at a heating rate of 5°C/min. The temperature of the GC/MS interface was 280°C, with the MS operated in the EI mode at 70 eV. The program was run in the scanning range from 29 to 400 a.m.u. at a rate of 2 scans/s. The identification of peaks was performed using the NISTMS library, with the area percents calibrated to compare the catalytic performance for the formation of valuable aromatic compounds. The experiments were conducted at least three times for each catalyst to confirm the reproducibility of the reported procedures. The average values of the peak area and peak area percent as received were calculated for each identified product. For the noncatalytic pyrolysis, only the L. japonica (2 mg) was placed in a sample cup and the same procedure with catalytic pyrolysis was applied.
Results and discussion
Characterization of L. japonica
Physicochemical properties of L. japonica
Proximate analysis (wt.%)
Ultimate analysis (wt.%)a
Characterization of catalysts
Textural properties of nanoporous catalysts
BET surface area (m2/g)a
Average pore size (nm)c
Noncatalytic pyrolysis using Py-GC/MS
The bio-oil quality can be evaluated through the chemical composition [1–13]. Many researchers have classified the different bio-oil organic compounds into desirables, such as phenolics, alcohols, and hydrocarbons, and undesirables, such as acids, carbonyls, polycyclic aromatic hydrocarbons (PAHs), and heavier oxygenates [1–13]. Generally, these undesirable compounds should be removed because oxygenates such as carbonyls and acids are responsible for many side-reactions during storage. In addition, most PAHs are well-known toxic and mutagenic compounds, whereas mono aromatics, such as benzene, toluene, ethyl benzene, and xylenes, can be considered highly valuable chemicals due to their commercial applicability in the petrochemical industry. Also, phenolics are useful materials because it can be used for phenolic resin and petrochemicals.
Selected main components of bio-oil produced by pyrolysis of L. japonica
In this study, more aromatic compounds were generated when Meso-MFI, which has strong Brönsted acid sites, was used compared to the case where Al-MCM-48 with weak acid sites was used. It can be suggested that some heavy compounds in the oil would react on the surface of the Meso-MFI catalyst and generate light hydrocarbons, such as ethylene and propylene. These light hydrocarbons then subsequently enter the pore of the Meso-MFI and undergo further polymerization and aromatization to form aromatic hydrocarbons. Also, similar results were reported from catalytic cracking over various catalysts: paraffinic hydrocarbons were the main products when nanoporous weak acidic Al-SBA-15 and Al-MCM-41 were used; whereas, the use of strong acidic HZSM-5 resulted in high yields of aromatic compounds . In our results, Al-MCM-48 also produced higher hydrocarbon than Meso-MFI.
In addition, the high acidity could affect the production of gases [17, 18]. Stronger acid sites can crack large molecules derived by thermal decomposition of L. japonica more easily, resulting in higher gas yields. Therefore, the use of strong acidic Meso-MFI resulted in a larger gas yield. Meanwhile, some amounts of undesirable PAHs due to its toxicity were produced for the catalytic upgrading. The high production of phenolics also may be ascribed to high acidity and large pore size of Meso-MFI. Heavy phenolics can be cracked into many small sizes of phenolics inside pore of Meso-MFI.
Nanoporous catalysts, Meso-MFI and Al-MCM-48, were used for the catalytic pyrolysis of L. japonica using Py-GC/MS. Bio-oil was converted to valuable products over nanoporous catalysts. In particular, Meso-MFI showed higher catalytic decomposition ability than Al-MCM-48. Meso-MFI produced high yields of aromatics, phenolics, and gases due to its strong acidic sites which accelerate cracking of pyrolyzed bio-oil molecules.
temperature programmed desorption of ammonia
pyrolysis gas chromatography/mass spectrometry
This research was supported by Basic Science Research Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Education, Science and Technology (no. 2009-0072328).
- Heo HS, Park HJ, Park YK, Ryu C, Suh DJ, Suh YW, Yim JH, Kim SS: Bio-oil production from fast pyrolysis of waste furniture sawdust in a fluidized bed. Bioresour Technol 2010, 101: S91-S96. 10.1016/j.biortech.2009.06.003View Article
- Park HJ, Heo HS, Park YK, Yim JH, Jeon JK, Park J, Ryu C, Kim SS: Clean bio-oil production from fast pyrolysis of sewage sludge: effects of reaction conditions and metal oxide catalysts. Bioresour Technol 2010, 101: S83-S85. 10.1016/j.biortech.2009.06.103View Article
- Heo HS, Park HJ, Yim JH, Sohn JM, Park J, Kim SS, Ryu C, Jeon JK, Park YK: Influence of operation variables on fast pyrolysis of Miscanthus sinensis var. purpurascens . Bioresour Technol 2010, 101: 3672–3677. 10.1016/j.biortech.2009.12.078View Article
- Heo HS, Park HJ, Park SH, Kim S, Suh DJ, Suh YW, Kim SS, Park YK: Fast pyrolysis of rice husks under different reaction conditions. J Ind Eng Chem 2010, 16: 27–31.View Article
- Bae YJ, Ryu C, Jeon JK, Park J, Suh DJ, Suh YW, Chang D, Park YK: The characteristics of bio-oil produced from the pyrolysis of three marine macroalgae. Bioresour Technol 2011, 102: 3512–3520. 10.1016/j.biortech.2010.11.023View Article
- Heo HS, Kim SG, Jeong KE, Jeon JK, Park SH, Kim JM, Kim SS, Park YK: Catalytic upgrading of oil fractions separated from food waste leachate. Bioresour Technol 2011, 102: 3952–3957. 10.1016/j.biortech.2010.11.099View Article
- Tran NH, Bartlett JR, Kannangara GSK, Milev AS, Volk H, Wilson MA: Catalytic upgrading of biorefinery oil from micro-algae. Fuel 2010, 89: 265–274. 10.1016/j.fuel.2009.08.015View Article
- Park HJ, Heo HS, Yim JH, Jeon JK, Ko YS, Kim SS, Park YK: Catalytic pyrolysis of Japanese larch using spent HZSM-5. Korean J Chem Eng 2010, 27: 73–75. 10.1007/s11814-009-0344-yView Article
- Park KH, Park HJ, Kim J, Ryu R, Jeon JK, Park J, Park YK: Application of hierarchical MFI zeolite for the catalytic pyrolysis of Japanese larch. J Nanosci Nanotechnol 2010, 10: 355–359. 10.1166/jnn.2010.1537View Article
- Park HJ, Heo HS, Jeon JK, Kim J, Ryoo R, Jeong KE, Park YK: Highly valuable chemicals production from catalytic upgrading of radiata pine sawdust-derived pyrolytic vapors over mesoporous MFI zeolites. Appl Catal B: Environmental 2010, 95: 365–373. 10.1016/j.apcatb.2010.01.015View Article
- Lee HI, Park HJ, Park YK, Hur JY, Jeon JK, Kim JM: Synthesis of highly stable mesoporous aluminosilicates from commercially available zeolites and their application to the pyrolysis of woody biomass. Catal Today 2008, 132: 68–74. 10.1016/j.cattod.2007.12.029View Article
- Park HJ, Jeon JK, Kim JM, Lee HI, Yim JH, Park JH, Park YK: Synthesis of nanoporous material from zeolite USY and catalytic application to bio-oil conversion. J Nanosci Nanotechnol 2008, 8: 5439–5444. 10.1166/jnn.2008.1102View Article
- Adam J, Blazso M, Meszaros E, Stocker M, Nilsen MH, Bouzga A, Hustad JE, Gronli M, Oye G: Pyrolysis of biomass in the presence of Al-MCM-41 type catalysts. Fuel 2005, 84: 1494–1502.
- Kim DI, Park JH, Kim SD, Lee JY, Yim JH, Jeon JK, Park SH, Park YK: Comparison of removal ability of indoor formaldehyde over different materials functionalized with various amine groups. J Ind Eng Chem 2011, 17: 1–5. 10.2298/CICEQ100216043BView Article
- Lee SH, Heo HS, Jeong KE, Yim JH, Jeon JK, Jung KY, Ko YS, Kim SS, Park YK: Catalytic pyrolysis of oilsand bitumen over nanoporous catalysts. J Nanosci Nanotechnol 2011, 11: 759–762. 10.1166/jnn.2011.3232View Article
- Lee HI, Kim JM, Lee JY, Park YK, Jeon JK, Yim JH, Park SH, Lee KJ, Kim SS, Jeong KE: Catalytic conversion of 1,2-dichlorobenzene over mesoporous materials from zeolite. J Nanosci Nanotechnol 2010, 10: 3639–3642. 10.1166/jnn.2010.2295View Article
- Choi SJ, Park YK, Jeong KE, Kim TW, Chae HJ, Park SH, Jeon JK, Kim SS: Catalytic degradation of polyethylene over SBA-16. Korean J Chem Eng 2010, 27: 1446–1451. 10.1007/s11814-010-0281-9View Article
- Park JH, Heo HS, Park YK, Jeong KE, Chae HJ, Sohn JM, Jeon JK, Kim SS: Catalytic degradation of high-density polyethylene over SAPO-34 synthesized with various templates. Korean J Chem Eng 2010, 27: 1768–1772. 10.1007/s11814-010-0282-8View Article
- Klyachko AL, Kapustin GI, Brueva TR, Rubinstein AM: Relationship between acidity and catalytic activity of high-silica zeolites in cracking. Zeolites 1987, 7: 119–122. 10.1016/0144-2449(87)90071-6View Article
- Katada N, Suzuki K, Noda T, Miyatani W, Taniguchi F, Niwa M: Correlation of the cracking activity with solid acidity and adsorption property on zeolites. Appl Catal A: Gen 2010, 373: 208–213. 10.1016/j.apcata.2009.11.022View Article
- Lukyanov DB, Gnep NS, Guisnet MR: Kinetic modeling of propane aromatization reaction over HZSM-5 and GaHZSM-5. Ind Eng Chem Res 1995, 34: 516–523. 10.1021/ie00041a012View Article
- Ooi YS, Zakaria R, Mohamed AR, Bhatia S: Catalytic conversion of fatty acids mixture to liquid fuel and chemicals over composite microporous/mesoporous catalysts. Energy Fuel 2005, 19: 736–743. 10.1021/ef049772xView Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.